Pressure-induced structural deformation and elastic...
Embed Size (px)
Transcript of Pressure-induced structural deformation and elastic...
American Mineralogist, Volume 93, pages 5362, 2008
0003-004X/08/0001053$05.00/DOI: 10.2138/am.2008.2554 53
* E-mail: email@example.com
Pressure-induced structural deformation and elastic behavior of wairakite
SIlvIa orI,1 SImona QuartIerI,2,* GIovanna vezzalInI,1 and vladImIr dmItrIev3
1Dipartimento di Scienze della Terra, Universit di Modena e Reggio Emilia, via S. Eufemia 19, 41100 Modena, Italy2Dipartimento di Scienze della Terra, Universit di Messina, Salita Sperone 31, 98166 Messina S. Agata, Italy
3Swiss-Norwegian Beam Lines at ESRF, BP220, 38043 Grenoble Cedex, France
abStractThe elastic behavior and the high-pressure structural evolution of the zeolite wairakite [ideal
chemical formula Ca(Al2Si4O12)2H2O, space group I2/a], the Ca-analog of analcime, have been investigated by means of in-situ synchrotron X-ray powder diffraction from ambient pressure to 7.8 GPa, and upon decompression. No complete X-ray amorphization is observed up to the highest investigated pressure, and the original unit-cell parameters are recovered upon decompression. The Rietveld structural refinements of the powder patterns converged successfully up to 2.5 GPa; above this pressure, a phase transition to triclinic symmetry is observed and only the unit-cell parameters were refined. An overall reduction of about 14% of the unit-cell volume between 0.0001 and 7.0 GPa is observed, demonstrating that wairakite is much more flexible upon compression than upon heating. The pressure dependence of the cell parameters is strongly anisotropic and larger after the transition to the triclinic space group. The elastic parameters refined with a second-order Birch-Murnaghan Equation of State are V0 = 2536(4) 3, K0 = 39(3) GPa, and V0 = 2632(38) 3, K0 = 24(3) GPa, for the monoclinic and triclinic phases, respectively.
The structure distortion of monoclinic wairakite, proceeding via tetrahedral tilting, induces deforma-tions in the 4-, 6-, and 8-membered rings and an increase in the extra-framework Ca coordination num-ber. A comparative discussion of the compressibility behavior of wairakite and analcime is reported.
Keywords: HP studies, XRD data, crystal structure, wairakite, phase transition, compressibility measurements
IntroductIonWairakite [ideal formula Ca(Al2Si4O12)2H2O] is an uncom-
mon zeolite first found by Steiner (1955) at Wairakei (New Zealand) and described as the Ca-analog of analcime. It occurs widely in low-grade metamorphic rocks, sedimentary environ-ments, and hydrothermal areas (Gottardi and Galli 1985; Tscher-nich 1992; Bish and Ming 2001). Wairakite forms a continuous solid solution series with analcime [Na2(Al2Si4O12)2H2O], and this name applies to the zeolites with ANA structural type (Baer-locher et al. 2001) with Ca as the most abundant extra-framework cation (Coombs et al. 1997). The same topology ANA is also shared by leucite, pollucite, hsianghualite, and several synthetic phases (Baerlocher et al. 2001).
The structurally related zeolite analcime has been described in a variety of different symmetries from cubic to triclinic. Sev-eral authors (Mazzi and Galli 1978; Hazen and Finger 1979) suggested that the reason for such of wide range of symmetries could be a different Si/Al distribution. Concerning wairakite, its crystal structure was determined by Takeuchi et al. (1979) on a monoclinic sample from Onikobe (Japan) in the space group I2/a. Henderson et al. (1998) determined the structure of the synthetic
counterpart by means of Rietveld analysis. The thermal stability and high-temperature (HT) behavior
of wairakite was studied by Seryotkin et al. (2003) by means of single-crystal X-ray diffraction and detailed structural informa-tion is available in the range between 20 and 600 C. The main feature is the reversible phase transformation, at about 150 C, from monoclinic I2/a to tetragonal I41/acd, with no fundamental change of the framework.
The only previous study of the high-pressure (HP) stability of wairakite was performed by Goryainov et al. (1999) with Raman spectroscopy on a single crystal mounted in a diamond anvil cell, using both water and glycerol as pressure transmitting media. These authors observed three phase transitions at 17.5, 31.3, and 67.0 kbar, interpreted as due to a decrease of the crystal symmetry along the sequence I2/a, P21/a, P1, P1. In particular, significant variations in shape and position of the bands related to O-T-O vibrational modes were observed upon compression. Significant broadening of bands and nonreversal of the P-induced transitions were attributed to amorphization, which was complete at about 82 kbar. Some other HP data are reported by the same authors (Goryainov et al. 1996) for dehydrated wairakite studied with the same spectroscopic technique. In this case, an irrevers-ible phase transition occurs at 34 kbar, attributed to polyhedral tilting. However, no details on any compressed crystal structure
ORI ET AL.: HP BEHAVIOR OF WAIRAKITE54
are available. The aim of this work is to investigate the elastic behavior
and the HP-structural evolution of wairakite by means of in-situ synchrotron X-ray powder diffraction (XRPD). Our results will be compared with those obtained on analcime (Gatta et al. 2006) to single out the influence of the Si/Al ordering and the type of extra-framework cation on the compressibility and on the HP deformation mechanisms of these isotypic zeolites. Moreover, the structural behavior of wairakite under HP and HT will be compared.
WaIrakIte cryStal StructureIn the wairakite structure (Takeuchi et al. 1979), described by
Gottardi and Galli (1985) as formed by singly connected 4-ring chains, two secondary building units are recognized: four- and six-membered rings of tetrahedra. The maximum symmetry of ANA topology is Ia3d. Two channel systems are present: irregular channels formed by distorted eight-membered rings along , and regular channels formed by six-membered rings along the  direction. The framework symmetry is lowered to the space group I2/a by the distribution of the extra-framework cations Ca and by the Al ordering on two preferred tetrahedra (T2A and T2B) (Takeuchi et al. 1979). The Al fractions of these two tetrahedra are identical. Among the extra-framework sites, two are fully occupied by water molecules and four by cations. Only one of these cation sites (M2) is almost completely occu-pied by Ca, while the others (M1, M12A, M12B) show a very low occupancy of Na. Wairakite and analcime present the same coordination geometry of the extra-framework cation polyhedra, which are regular octahedra formed by two water molecules at the apices and four framework O atoms belonging to the two tetrahedra mainly centered by Al.
experImental methodSWairakite used in this study comes from the type locality Wairakei (New
Zealand) (Steiner 1955). The electron microprobe analysis was carried out at the Earth Science Department of University of Modena and Reggio Emilia, using an ARL-SEMQ instrument in wavelength dispersive mode, operating at 15 kV and with a beam current of 20 nA and diameter of 20 m. The standards used were Amelia albite for Si, Al, and Na, AB microcline for K, paracelsian for Ba, and synthetic Di85-JD15, AN70 glass, Sr-anorthite, and P140 olivine for Mg, Ca, Sr, and Fe, respectively. The data acquisition and processing were performed using the PROBE program (Donovan 1995). The water content is from Steiner (1955). The corresponding formula is (Ca7.12Na1.21K0.03Sr0.02) (Al15.74Si32.31O96)16.43 H2O. The unit-cell parameters determined at ambient conditions on the powder inside the DAC are a = 13.6921(5) , b = 13.6500(4) , c = 13.5672(3) , = 90.508(3), and V = 2535.56 (8) 3.
Synchrotron X-ray powder diffraction experimentsThe high-pressure XRPD experiments were performed at the SNBL1 (BM01a)
beamline at European Synchrotron Radiation Facility (ESRF) with fixed wave-length of 0.7 , using a modified Merril-Bassett DAC (Miletich et al. 2000) and silicone oil as the non-penetrating P-transmitting medium. These conditions were chosen to allow the comparison of wairakite compressibility with those of the other zeolites studied by our group using the same non-penetrating P-transmitting medium (Vezzalini et al. 2001; Ballone et al. 2002; Ferro et al. 2002; Arletti et al. 2003; Fois et al. 2005a, 2005b; Betti et al. 2007). The pressure was measured using the ruby fluorescence method (Forman et al. 1972) on the non-linear hydrostatic pressure scale (Mao et al. 1986). The estimated error in the pressure values is 0.1 GPa. A MAR345 detector (pixel dimension 150 m) was used at a fixed distance of 230 mm from the sample; the exposure time was 120 s for all pressure points. One-dimensional diffraction patterns were obtained in the 2 range 047 by integrating the two dimensional images with the program FIT2D (Hammersley et al. 1996)
and are reported in Figure 1. The experiments were performed from ambient pressure (Pamb) up to 7.8 GPa,
with P increments of 0.20.6 GPa. Sample was equilibrated for about 30 min at each measured pressure. Three other patterns were collected while decompressing the sample up to Pamb [5.7 (rev), 3.4 (rev), Pamb(rev), in the following and in tables]. As a whole, 27 spectra were collected.
Lattice parameters and structural refinements strategyDue to the low quality of the powder patterns collected in the highest-pressure
regime, the data analysis was performed only up to 7.0 GPa. Two different strategies were adopted in the two ranges Pamb2.5 and 3.27.0 GPa, whereas in the first P range complete Rietveld structural refinements were performed, above 2.5 GPa a P-induced symmetry lowering was observed and only the unit-cell values were extracted from the diffraction patterns.
The Rietveld profile fit